常规环氧地坪漆施工工序：1、地面打磨清理干净，无尘打磨机打磨；2、涂刷高效环氧地坪漆底漆，根据不同的地面做不同的环氧地坪漆底漆，地面情况不同，环氧地坪漆底漆耗漆量也不一样，新地面环氧地坪漆耗漆量通常是0.15kg/㎡左右，起砂严重的地面环氧地坪漆耗量则可达 0.5kg/㎡以上；3、环氧地坪漆底漆固化之后，涂刷无溶剂环氧环氧地坪漆中涂，根据地面环氧环氧地坪漆涂刷道数，每平米环氧地坪漆耗漆量 0.3kg/㎡；
Conventional construction procedures of epoxy floor paint: 1. Clean up the ground and polish with dust-free grinder; 2. Paint high-efficiency epoxy floor paint primer, make different epoxy floor paint primers according to different ground conditions, the amount of epoxy floor paint primer consumption is different, the amount of new ground epoxy floor paint consumption is usually 0.1. The consumption of epoxy flooring paint with serious sand rising can reach 0.5kg/or above at 5kg/. 3. After curing, epoxy flooring paint is coated with solvent-free epoxy flooring paint. According to the number of brushing paths of epoxy flooring paint, the consumption of epoxy flooring paint is 0.3kg/per square meter.
4. Apply epoxy putty to fill the seam. The paint consumption of epoxy floor paint is 0.2kg/.
5、刮涂两遍环氧地坪漆面漆，环氧地坪漆耗漆量 0.3kg/㎡，自流平面漆是先刮涂一道环氧地坪漆，然后再镘涂一道环氧地坪漆，耗漆量为 1.1kg/㎡；
5. Scrape two times of epoxy floor paint, the consumption of epoxy floor paint is 0.3 kg/. Self-flow floor paint is to scrape an epoxy floor paint first, then apply an epoxy floor paint, the consumption of paint is 1.1 kg/.
6. In order to prevent the wear and tear of epoxy flooring paint film, one can apply a varnish epoxy flooring paint to self-leveling after painting the epoxy flooring paint, which can better prevent the long-term friction and tear of the epoxy flooring paint film and effectively prolong the service life of the flooring.
Basic process of epoxy floor paving
（0） 面涂批补：采用面涂材料配石英细粉批涂，填补中涂较大颗粒间的空隙，待完全固化后，用无尘打磨机打磨地面，用吸 尘器吸尽灰尘、打磨平整。
(0) Surface painting batch repairing: using surface coating material with quartz powder batch coating, filling the gap between larger particles in the middle coating, to be fully solidified, using dust-free grinder to grind the ground, using a vacuum cleaner to absorb dust, grinding flat.
(1) Base treatment: grinding loose layer, delamination and cement residue to make it hard and smooth, and increase the adhesion between the floor coating and the ground.
(2) Primer construction: After the epoxy sealing primer is matched, roll, scrape or brush are applied to wet the concrete fully and infiltrate into the inner layer of the concrete.
(3) Intermediate coating construction: mix the middle coating material with appropriate amount of quartz sand and mix evenly, and coat it with trowel to form a uniform and compact layer with a certain thickness.
（4） 面涂批补：采用面涂材料配石英细粉批涂，填补中涂较大颗粒间的空隙，待完全固化后，用无尘打磨机打磨地面，用吸 尘器吸尽灰尘、打磨平整。
(4) Surface painting batch repairing: using surface coating material with quartz powder batch coating, filling the gap between the larger particles in the middle coating, to be fully solidified, using dust-free grinder to grind the ground, using a vacuum cleaner to absorb dust, grinding flat.
(5) Surface coating construction: After mixing epoxy paint and curing agent evenly, it can be sprayed, brushed, rolled or sprayed to make it level and obtain a smooth and uniform surface coating.
Plant floor epoxy floor paint construction steps:
1. Base surface cleaning: While grinding rough basement surface with a motor grinder, then using a manual grinder to remove the basement that needs to be thoroughly cleaned;
2. Clean and check the base: After cleaning the base surface, check whether there are cracks and empty shells in the base. If so, it must be cut deep and filled with epoxy resin mortar. Because the epoxy resin is not water-tolerant, it can only be dry treated in the process of cleaning, so it can not be brutally knocked when cleaning, so as to avoid loosening the base on the edge.
3. Epoxy resin primer coating: epoxy primer coating can be carried out at the same time as the base treatment. The balance between construction progress and materials should be paid attention to during construction proportioning, so as to ensure that the material still meets the usable time in painting and is painted before gelatinization, so as to maintain good permeability of the material, and ensure that the material can not be overloaded at one time. Adhesive property;
4. After solidification of the primer, the epoxy resin is first coated with quartz sand to scrape the epoxy quartz mortar N times, so as to increase the thickness of the whole film and enhance the physical properties of the film, such as compression and impact resistance.
5. Epoxy resin batch soil coating: after curing the mortar layer, scrape the epoxy batch soil 2 ways, seal sand holes and stomata, Polish putty and dust clean.
6. Epoxy resin surface coating: coating in polishing, in order to ensure that the base surface is completely closed, two epoxy resin flat coatings should be constructed according to the design requirements, and the surface coating materials should be stirred evenly before rolling coating construction; the environmental requirements of coating construction: the construction base surface should be kept clean and dry, and there is no cross-work of other engineering construction. Industry, indoor air relative humidity should be less than 85%, when humidity is too large, we should stop construction.
7. On-site cleaning and maintenance, floor maintenance: After finishing the surface painting, the relevant construction materials and tools will be removed from the site, and the finish decoration will be tightly sealed and protected. At least 48 hours later, people can be allowed to walk. No sediment should be brought in. It usually takes 7 days to solidify the paint film completely. During this period, other engineering construction, handling and installation should be avoided.
标签:   环氧地坪 地坪 环氧地坪漆 环氧地坪施工